3CastingRefractory mold pour liquid metal solidify, remove finishVERSATILE: complex geometry, internal cavities, hollow sectionsVERSATILE: small (~10 grams) very large parts (~1000 Kg)ECONOMICAL: little wastage (extra metal is re-used)ISOTROPIC: cast parts have same properties along all directions
4Different Casting Processes AdvantagesDisadvantagesExamplesSandmany metals, sizes, shapes, cheappoor finish & toleranceengine blocks, cylinder headsShell moldbetter accuracy, finish, higher production ratelimited part sizeconnecting rods, gear housingsExpendablepatternWide range of metals, sizes, shapespatterns have low strengthcylinder heads, brake componentsPlaster moldcomplex shapes, good surface finishnon-ferrous metals, low production rateprototypes of mechanical partsCeramic moldcomplex shapes, high accuracy, good finishsmall sizesimpellers, injection mold toolingInvestmentcomplex shapes, excellent finishsmall parts, expensivejewelleryPermanent moldgood finish, low porosity, high production rateCostly mold, simpler shapes onlygears, gear housingsDieExcellent dimensional accuracy, high production ratecostly dies, small parts,non-ferrous metalsgears, camera bodies, car wheelsCentrifugalLarge cylindrical parts, good qualityExpensive, few shapespipes, boilers, flywheels
7Sand Casting Considerations (a) How do we make the pattern?[cut, carve, machine](b) Why is the pattern not exactly identical to the part shape?- pattern outer surfaces; (inner surfaces: core)- shrinkage, post-processing(c) parting line- how to determine?
8Sand Casting Considerations.. (d) taper- do we need it ?(e) core prints, chaplets- hold the core in position- chaplet is metal (why?)(f) cut-off, finishing
9Shell mold casting - metal, 2-piece pattern, 175C-370C - coated with a lubricant (silicone)- mixture of sand, thermoset resin/epoxy- cure (baking)- remove patterns, join half-shells mold- pour metal- solidify (cooling)- break shell part
10Expendable Mold Casting - Styrofoam pattern- dipped in refractory slurry dried- sand (support)- pour liquid metal- foam evaporates, metal fills the shell- cool, solidify- break shell part
11Plaster-mold, Ceramic-mold casting Plaster-mold slurry: plaster of paris (CaSO4), talc, silica flourCeramic-mold slurry: silica, powdered Zircon (ZrSiO4)- The slurry forms a shell over the pattern- Dried in a low temperature oven- Remove pattern- Backed by clay (strength), baked (burn-off volatiles)- cast the metal- break mold partPlaster-mold: good finish (Why ?)plaster: low conductivity => low warpage, residual stresslow mp metal (Zn, Al, Cu, Mg)Ceramic-mold: good finishhigh mp metals (steel, …) => impeller blades, turbines, …
12Investment casting (lost wax casting) (a) Wax pattern(injection molding)(b) Multiple patternsassembled to wax sprue(d) dry ceramicmelt out the waxfire ceramic (burn wax)(c) Shell built immerse into ceramic slurry immerse into fine sand(few layers)(e) Pour molten metal (gravity) cool, solidify[Hollow casting:pouring excess metal before solidification(f) Break ceramic shell(vibration or water blasting)(g) Cut off parts(high-speed friction saw) finishing (polish)
13Permanent mold casting MOLD: made of metal (cast iron, steel, refractory alloys)CORE: (hollow parts)- metal: core can be extracted from the part- sand-bonded: core must be destroyed to removeMold-surface: coated with refractory material- Spray with lubricant (graphite, silica)- improve flow, increase life- good tolerance, good surface finish- low mp metals (Cu, Bronze, Al, Mg)
14Die casting - a type of permanent mold casting - common uses: components forrice cookers, stoves, fans, washing-, drying machines,fridges, motors, toys, hand-tools, car wheels, …HOT CHAMBER: (low mp e.g. Zn, Pb; non-alloying)(i) die is closed, gooseneck cylinder is filled with molten metal(ii) plunger pushes molten metal through gooseneck into cavity(iii) metal is held under pressure until it solidifies(iv) die opens, cores retracted; plunger returns(v) ejector pins push casting out of ejector dieCOLD CHAMBER: (high mp e.g. Cu, Al)(i) die closed, molten metal is ladled into cylinder(ii) plunger pushes molten metal into die cavity(iii) metal is held under high pressure until it solidifies(iv) die opens, plunger pushes solidified slug from the cylinder(v) cores retracted(iv) ejector pins push casting off ejector die
15Centrifugal casting - permanent mold - rotated about its axis at 300 ~ 3000 rpm- molten metal is poured- Surface finish: better along outer diameter than inner,- Impurities, inclusions, closer to the inner diameter (why ?)
25Non-Consumable Electrode Fusion Welding ProcessesWelding ProcessesConsumable ElectrodeSMAW – Shielded Metal Arc WeldingGMAW – Gas Metal Arc WeldingSAW – Submerged Arc WeldingNon-Consumable ElectrodeGTAW – Gas Tungsten Arc WeldingPAW – Plasma Arc WeldingHigh Energy BeamTo be finishedElectron Beam WeldingLaser Beam Welding
26Welding Processes SMAW – Shielded Metal Arc Welding Consumable electrodeFlux coated rodFlux produces protective gas around weld poolSlag keeps oxygen off weld bead during coolingGeneral purpose welding—widely usedPower... Current I ( amps)Voltage V ( volts)Thicknesses 1/8” – 3/4”To be finishedPortablePower = VI 10 kW
27(–) (+) (+) (–) Welding Processes SMAW - DC Polarity Electric Arc Welding -- PolarityWelding ProcessesSMAW - DC PolarityStraight PolarityReverse Polarity(–)(+)(+)(–)Shallow penetrationDeeper weld penetrationTo be finished(thin metal)AC - Gives pulsing arc- used for welding thick sections
28Welding Processes GMAW – Gas Metal Arc Welding (MIG) DC reverse polarity - hottest arcAC - unstable arcGas Metal Arc Welding (GMAW) TorchMIG - Metal Inert GasConsumable wire electrodeTo be finishedShielding provided by gasDouble productivity of SMAWEasily automatedGroover, M., Fundamentals of Modern Manufacturing,, p. 734, 1996
29Welding Processes GMAW – Gas Metal Arc Welding (MIG) DC reverse polarity - hottest arcAC - unstable arcGas Metal Arc Welding (GMAW) TorchMIG - Metal Inert GasConsumable wire electrodeTo be finishedShielding provided by gasDouble productivity of SMAWEasily automatedGroover, M., Fundamentals of Modern Manufacturing,, p. 734, 1996
30Welding Processes SAW – Submerged Arc Welding 300 – 2000 amps (440 V) Consumable wire electrodeGas Metal Arc Welding (GMAW) TorchShielding provided by flux granulesLow UV radiation & fumesTo be finishedFlux acts as thermal insulatorAutomated process (limited to flats)High speed & quality (4 – 10x SMAW)Suitable for thick plates
31Welding Processes GTAW – Gas Tungsten Arc Welding (TIG) Power 8-20 kWCurrent I (200 A DC)(500 A AC)a.k.a. TIG - Tungsten Inert GasNon-consumable electrodeTo be finishedWith or without filler metalShield gas usually argonUsed for thin sections of Al, Mg, Ti.Most expensive, highest quality
32Welding Processes Friction Welding (Inertia Welding) One part rotated, one stationaryStationary part forced against rotating partFriction converts kinetic energy to thermal energyMetal at interface melts and is joinedWhen sufficiently hot, rotation is stopped & axial force increasedTo be finished
33Welding Processes Resistance Welding Resistance Welding is the coordinated application of electric current and mechanical pressure in the proper magnitudes and for a precise period of time to create a coalescent bond between two base metals.Heat provided by resistance to electrical current (Q=I2Rt)Typical 0.5 – 10 V but up to 100,000 amps!Force applied by pneumatic cylinderOften fully or partially automatedTo be finished- Spot welding- Seam welding
34Welding Processes Resistance Welding Heat provided by resistance to electrical current (Q=I2Rt)Typical 0.5 – 10 V but up to 100,000 amps!Force applied by pneumatic cylinderOften fully or partially automatedTo be finished- Spot welding- Seam welding
35Welding Processes Diffusion Welding Parts forced together at high temperature(< 0.5Tm absolute) and pressureHeated in furnace or by resistance heatingAtoms diffuse across interfaceAfter sufficient time the interface disappearsGood for dissimilar metalsTo be finishedBond can be weakened by surface impuritiesKalpakjian, S., Manufacturing Engineering & Technology, p. 889, 1992
36Metal Joining Processes Soldering & BrazingMetal Joining ProcessesSoldering & BrazingOnly filler metal is melted, not base metalLower temperatures than weldingFiller metal distributed by capillary actionMetallurgical bond formed between filler & base metalsStrength of joint typicallystronger than filler metal itselfweaker than base metalgap at joint important (0.001 – 0.010”)To be finishedPros & ConsCan join dissimilar metalsLess heat - can join thinner sections (relative to welding)Excessive heat during service can weaken joint
37Metal Joining Processes SolderingMetal Joining ProcessesSolderingSolder = Filler metalAlloys of Tin (silver, bismuth, lead)Melt point typically below 840 FFlux used to clean joint & prevent oxidationseparate or in core of wire (rosin-core)Tinning = pre-coating with thin layer of solderApplications:Printed Circuit Board (PCB) manufacturePipe joining (copper pipe)To be finishedJewelry manufactureTypically non-load bearingEasy to solder: copper, silver, goldDifficult to solder: aluminum, stainless steels(can pre-plate difficult to solder metals to aid process)
38Metal Joining Processes PCB SolderingMetal Joining ProcessesManual PCB SolderingSoldering Iron & Solder WireHeating lead & placing solderTo be finishedHeat for 2-3 sec. & place wire opposite ironTrim excess lead
39Metal Joining Processes PCB Reflow SolderingMetal Joining ProcessesAutomated Reflow SolderingSMT = Surface Mount TechnologySolder/Flux paste mixture applied to PCB using screen print or similar transfer methodSolder Paste serves the following functions:supply solder material to the soldering spot,hold the components in place prior to soldering,clean the solder lands and component leadsprevent further oxidation of the solder lands.Printed solder paste on a printed circuit board (PCB)PCB assembly then heated in “Reflow” oven to melt solder and secure connectionTo be finished
40Metal Joining Processes BrazingMetal Joining ProcessesBrazingUse of low melt point filler metal to fill thin gap between mating surfaces to be joined utilizing capillary actionFiller metals include Al, Mg & Cu alloys (melt point typically above 840 F)Flux also usedTypes of brazing classified by heating method:Torch, Furnace, ResistanceApplications:To be finishedAutomotive - joining tubesPipe/Tubing joining (HVAC)Electrical equipment - joining wiresJewelry MakingJoint can possess significant strength
41Metal Joining Processes BrazingMetal Joining ProcessesBrazingUse of low melt point filler metal to fill thin gap between mating surfaces to be joined utilizing capillary actionFiller metals include Al, Mg & Cu alloys (melt point typically above 840 F)Flux also usedTypes of brazing classified by heating method:Torch, Furnace, ResistanceApplications:To be finishedAutomotive - joining tubesPipe/Tubing joining (HVAC)Electrical equipment - joining wiresJewelry MakingJoint can possess significant strength
42Deformation Processes UNIT IIIDeformation Processes
43FormingAny process that changes the shape of a raw stockwithout changing its phaseExample products:Al/Steel frame of doors and windows, coins, springs,Elevator doors, cables and wires, sheet-metal, sheet-metal parts…
45RollingImportant Applications:Steel Plants,Raw stock production (sheets, tubes, Rods, etc.)Screw manufacture
46Rolling Basics Screw manufacture: Sheets are rolled in multiple stages (why ?)Screw manufacture:
47Forging[Heated] metal is beaten with a heavy hammer to give it the required shapeHot forging,open-die
48Stages in Open-Die Forging (a) forge hot billet to max diameter(b) “fuller: tool to mark step-locations(c) forge right side(d) reverse part, forge left side(e) finish (dimension control)[source:www.scotforge.com]
49Stages in Closed-Die Forging [source:Kalpakjian & Schmid]
50Quality of forged parts Surface finish/Dimensional control:Better than casting (typically)Stronger/tougher than cast/machined parts of same material[source:www.scotforge.com]
51Extrusion Metal forced/squeezed out through a hole (die) [source:www.magnode.com]Typical use: ductile metals (Cu, Steel, Al, Mg), Plastics, RubbersCommon products:Al frames of white-boards, doors, windows, …
52Extrusion: Schematic, Dies Exercise: how can we get hollow parts?
53DrawingSimilar to extrusion, except: pulling force is appliedCommonly used to make wires from round bars
62Sheet metal bendingPlanning problem: what is the sequence in which we do the bending operations?Avoid: part-tool, part-part, part-machine interference
63Bending mechanicsBending Planning what is the length of blank we must use?Ideal case: k = 0.5Real cases: k = 0.33 ( R < 2T) ~~ k = 0.5 (R > 2T)
64Bending: cracking, anisotropic effects, Poisson effect Bending plastic deformationEngineering strain in bending = e = 1/( 1 + 2R/T)Bending disallow failure (cracking) limits on corner radius: bend radius ≥ 3Teffect of anisotropic stockPoisson effectExercise: how does anisotropic behavior affect planning?
65How to handle springback: Bending: springbackInitialFinalRifafaiTHow to handle springback:(a) Compensation: the metal is bent by a larger angle(b) Coining the bend:at end of bend cycle, tool exerts large force, dwellscoining: press down hard, wait, release
66Deep Drawing Tooling: similar to punching operation, Mechanics: similar to bending operationCommon applications: cooking pots, containers, …
67Sheet metal parts with combination of operations Body of Olympus E-300 cameracomponent with multiple bending operationscomponent with punching,bending, drawing operations[image source: dpreview.com]
68SPECIAL WELDING AND FORMING PROCESS UNIT IVSPECIAL WELDING AND FORMING PROCESS
69THERMIT WELDINGThermit welding is a mixture of aluminium powder and metal oxide which when ignited results in a non explosive exothermic reaction. The heat so generated melts and reduces the metal oxide to metallic form at high temperature. This molten metal is used for joining metal parts by pouring it between them resulting in cast weld joint.
70Welding Processes Laser Welding Laser beam produced by a CO2 or YAG LaserHigh penetration, high-speed processConcentrated heat = low distortionLaser can be shaped/focused & pulsed on/offTypically automated & high speed (up to 250 fpm)Workpieces up to 1” thickTypical laser welding applications :Catheters & Other Medical DevicesSmall Parts and ComponentsFine WiresJewelrySmall SensorsThin Sheet Materials Down To 0.001" ThickTo be finished
71ULTRASONIC WELDINGIn ultrasonic welding a metallic tip vibrating at ultrasonic frequency is made to join a thin piece to a thicker piece supported on anvil. Frequency used is from 20khz to 60khz. Ultrasonic welding equipment consists of mainly two parts, one is power source and other is transducer.
72Explosive forming EXPLOSIVE FORMING First used to form metals in the 1900’s. A sheet metal blank is clamped over a die, and the entire assembly is lowered into a tank filled with water. The air in the cavity is evacuated, and an explosive is detonated at a certain height above.
73MAGNETIC PULSE FORMING Also called electromagnetic forming. Energy stored in a capacitor bank is discharged rapidly through a magnetic coil. Magnetic field crosses metal tube (conductor) creating eddy currents which have an opposing magnetic field.(b)(a)Figure (a) Schematic illustration of the magnetic-pulse forming process used to form a tube over a plug. (b) Aluminum tube collapsed over a hexagonal plug by the magnetic-pulse forming process.
7416.8 Rubber Forming Rubber Forming One of the dies in the set is made of polyurethane membrane, which is a type of flexible material.Polyurethane is resistant to abrasion, cutting or tearing by the metal, and has a long fatigue life.
7516.9 Spinning Conventional Spinning Process where a circular piece of sheet metal is placed and held against a mandrel and rotated while a rigid tool deforms and shapes the material over the mandrel.May be performed at room temperature or at higher temperature for thicker metal.
78Basic Steps In Powder Metallurgy (P/M) Powder ProductionBlending or MixingCompactionSinteringFinishing
79Powder Production Atomization the most common Others Chemical reduction of oxidesElectrolytic depositionDifferent shapes producedWill affect compaction process significantly
80Blending or MixingCan use master alloys, (most commonly) or elemental powders that are used to build up the alloysMaster alloys are with the normal alloy ingredientsElemental or pre-alloyed metal powders are first mixed with lubricants or other alloy additions to produce a homogeneous mixture of ingredientsThe initial mixing may be done by either the metal powder producer or the P/M parts manufacturerWhen the particles are blended:Desire to produce a homogenous blendOver-mixing will work-harden the particles and produce variability in the sintering process
81Compaction Usually gravity filled cavity at room temperature Pressed at ksiProduces a “Green” compactSize and shape of finished part (almost)Not as strong as finished part – handling concernFriction between particles is a major factor
82Isostatic Pressing Because of friction between particles Apply pressure uniformly from all directions (in theory)Wet bag (left)Dry bag (right)
83Sintering Parts are heated to ~80% of melting temperature Transforms compacted mechanical bonds to much stronger metal bondsMany parts are done at this stage. Some will require additional processing
84Sintering ctd Final part properties drastically affected Fully sintered is not always the goalIe. Self lubricated bushingsDimensions of part are affected
85Die Design for P/M Thin walls and projections create fragile tooling. Holes in pressing direction can be round, square, D-shaped, keyed, splined or any straight-through shape.Draft is generally not required.Generous radii and fillets are desirable to extend tool life.Chamfers, rather the radii, are necessary on part edges to prevent burring.Flats are necessary on chamfers to eliminate feather-edges on tools, which break easily.
86Advantages of P/MVirtually unlimited choice of alloys, composites, and associated propertiesRefractory materials are popular by this processControlled porosity for self lubrication or filtration usesCan be very economical at large run sizes (100,000 parts)Long term reliability through close control of dimensions and physical propertiesWide latitude of shape and designVery good material utilization
87Disadvantages of P/M Limited in size capability due to large forces Specialty machinesNeed to control the environment – corrosion concernWill not typically produce part as strong as wrought product. (Can repress items to overcome that)Cost of die – typical to that of forging, except that design can be more – specialtyLess well known process
88Financial Considerations Die design – must withstand 100 ksi, requiring specialty designsCan be very automated1500 parts per hour not uncommon for average size part60,000 parts per hour achievable for small, low complexity parts in a rolling pressTypical size part for automation is 1” cubeLarger parts may require special machines (larger surface area, same pressure equals larger forces involved)
89Manufacturing of Plastic Components UNIT VManufacturing of Plastic Components
90ExtrusionRaw materials in the form if thermoplastic pallets,granules,or powder, placed into a hopper and fed into extruder barrel.The barrel is equipped with a screw that blends the pallets and conveys them down the barrelHeaters around the extruder’s barrels heats the pellets and liquefies themScrew has 3-sectionsFeed sectionMelt or transition sectionPumping section.
91Complex shapes with constant cross-section Solid rods, channels, tubing, pipe, window frames, architectural components can be extruded due to continuous supply and flow.Plastic coated electrical wire, cable, and strips are also extrudedPellets :extruded product is a small-diameter rod which is chopped into small pelletsSheet and film extrusion :Extruded parts are rolled on water and on the rollers
92ExtruderFig : Schematic illustration of a typical extruder for plastics, elastomers, and composite materials.
93Injection moldingFig : Injection molding with (a) plunger, (b) reciprocating rotating screw, (c) a typical part made from an injection molding machine cavity, showing a number of parts made from one shot, note also mold features such as sprues, runners and gates.
94Similar to extrusion barrel is heated Pellets or granules fed into heated cylinderMelt is forced into a split-die chamberMolten plastic pushed into mold cavityPressure ranges from 70 Mpa – 200 MpaTypical products : Cups, containers, housings, tool handles, knobs, electrical and communication components, toys etc.
95Injection moldingInjection molds have several components such as runners, cores, cavities, cooling channels, inserts, knock out pins and ejectors3-basic types of moldsCold runner two plate moldCold runner three plate moldHot runner moldFig : Examples of injection molding
96Injection Molding Machine Fig : A 2.2-MN (250-ton) injection molding machine. The tonnage is the force applied to keep the dies closed during injection of molten plastic into the mold cavities.
97Process capabilities : High production ratesGood dimensional controlCycle time range 5 to 60 sec’sMold materials- tool steels, beryllium - Cu, AlMold life- 2 million cycles (steel molds)10000 cycles ( Al molds)Machines :Horizontal or vertical machinesClamping – hydraulic or electric
98Blow molding Modified extrusion and Injection Molding process. A tube extruded then clamped to mold with cavity larger than tube diameter.Finally blown outward to fill the cavityPressure 350Kpa-700KpaOther Blow Molding processesInjection Blow moldingMulti layer Blow molding
99Fig : Schematic illustration of (a) the blow-molding process for making plastic beverage bottles, and (b) a three-station injection blow-molding machine.
100Rotational MoldingThermo plastics are thermosets can be formed into large parts by rotational moldingA thin walled metal mold is made of 2 piecesRotated abut two perpendicular axesPre-measured quantity of powdered plastic material is rotated about 2-axesTypical parts produced-Trash cans, boat hulls, buckets, housings, toys, carrying cases and foot balls.
101Rotational MoldingFig: The rotational molding (rotomolding or rotocasting) process. Trash cans, buckets, and plastic footballs can be made by this process.
102ThermoformingSeries process for forming thermoplastic sheet or film over a mold by applying heat and pressure.Typical parts : advertising signs, refrigerator liner, packaging , appliance housing, and panels for shower stalls .Fig : Various Thermoforming processes for thermoplastic sheet. These processes are commonly used in making advertising signs, cookie and candy trays, panels for shower stalls, and packaging.
103Compression moldingPre-shaped charge ,pre-measured volume of powder and viscous mixture of liquid resin and filler material is placed directly into a heated mold cavity.Compression mold results in a flash formation which is a n excess material.Typical parts made are dishes, handles, container caps fittings, electrical and electronic components and housingsMaterials used in compression molding are thermosetting plastics & elastomersCuring times range from 0.5 to 5 mins3- types of compression molds areFlash typePositive typeSemi-positive
104Compression MoldingFig : Types of compression molding, a process similar to forging; (a) positive, (b) semi positive, (c) flash (d) Die design for making compression-molded part with undercuts.
105Transfer moldingTransfer molding is an improvement if compression moldingUncured thermosetting material placed in a heated transfer pot or chamber, which is injected into heated closed moldsRam plunger or rotating screw feeder forces material into mold cavity through narrow channelsThis flow generates heat and resin is molten as it enters the moldTypical parts : Electrical & electronic components, rubber and silicone parts
106Transfer moldingFig : Sequence of operations in transfer molding for thermosetting plastics. This process is particularly suitable for intricate parts with varying wall thickness.
107Casting Fig : Casting Conventional casting of thermo plastics : Mixture of monomer, catalyst and various additives are heated and poured into the mouldThe desired part is formed after polymerization takes place.Centrifugal casting :Centrifugal force used to stack the material onto the moldReinforced plastics with short fibers are usedFig : Casting
108Cold forming Solid Phase forming Processes such as rolling ,deep drawing extrusion closed die forging ,coining and rubber forming can be used for thermoplastics at room temperaturesTypical materials used : Poly propylene, poly carbonate, Abs, and rigid PVCConsiderations :Sufficiently ductile material at room temperatureNon recoverable material deformationSolid Phase formingTemperatures from 10oc to 20oc are maintained, which is below melting pointAdvantages :Spring-back is lowerDimensional accuracy can be maintained
109Calendaring and Examples of Reinforced Plastics Fig : Schematic illustration of calendaring, Sheets produced by this process are subsequently used in thermoforming.Fig : Reinforced-plastic components for a Honda motorcycle. The parts shown are front and rear forks, a rear swing arm, a wheel, and brake disks.
110Sheet MoldingFig : The manufacturing process for producing reinforced-plastic sheets. The sheet is still viscous at this stage; it can later be shaped into various products.
111Examples of Molding processes Fig : (a) Vacuum-bag forming. (b) Pressure-bag forming.Fig : Manual methods of processing reinforced plastics: (a) hand lay-up and (b) spray-up. These methods are also called open-mold processing.